39.2: optical analysis of vertical aligned mode on 39.2 / b. l. zhang 39.2: optical analysis of...
Click here to load reader
Post on 27-Jun-2020
Embed Size (px)
39.2 / B. L. Zhang
39.2: Optical Analysis of Vertical Aligned Mode on Color Filter Liquid-Crystal-on-Silicon Microdisplay
B. L. Zhang, H. S. Kwok, and H. C. Huang Centre for Display Research, Hong Kong University of Science and Technology, Clear Water Bay, Hong Kong
Y. C. Chen Himax Display, No.12, Nanke 8th Road, Tainan Science-based Industrial Park, Tainan, Taiwan
Abstract We report our studies of vertical aligned mode on color filter liquid-crystal-on-silicon microdisplay. Three-dimensional optical analyses were performed to minimize fringing field effect in small color pixels. The simulation results were compared with experimental data and also the results of twisted nematic mode. 1. Introduction We have developed a color filter liquid-crystal-on-silicon (CF- LCOS) microdisplay that integrated color filters on silicon. In our previous works, we have presented process, characterization and optical modeling of this breed of CF-LCOS microdisplays in twisted nematic (TN) mode [1, 2]. We used either rubbed or photo-aligned method  for these microdisplays, and they worked well for near-to-eye or mini-projector which had light illumination below 8 million lux. However, the display performance started to degrade when the light illumination exceed 15 million lux. The color filter can still resist strong light illumination. But the rubbed or photo-aligned layer was suffered from strong light illumination, especially the ultra-violet part of the light, and the contrast and color saturation of the display was accordingly degraded. In this paper, we report our studies of vertical aligned (VA) mode on the CF-LCOS microdisplays. The use of inorganic silicon oxide as the alignment layer could improve light stability of the microdisplays. We therefore applied this technology to CF-LCOS microdisplays, and at the same time, configured the microdisplays to VA mode for better contrast . Three-dimensional optical analyses were performed to analyse and optimize these VA CF- LCOS microdisplays, and also provided guidelines for experiments.
2. Process of VA CF-LCOS Microdisplays The assembly process of the VA mode is very similar to that of the conventionally TN mode, except the alignment layer. Though there are special polyimide layers that can be spun and coated on the silicon or glass substrate as the alignment layer for the VA mode [5, 6]. Their pretilt angles were limited and they had light stability problem due to the polyimide base alignment layer. Therefore, at present, the majority of the LCOS microdisplays of VA mode used the silicon oxide as the alignment layer [7-11]. In the process of the CF-LCOS microdisplay of the VA mode, the silicon oxide was also adopted as the alignment layer. The color filter silicon substrate was prepared by the same process as reported in our previous works . The color filter array was again 0.75μm for all three colors. Then, a thin layer of silicon oxide was sputtered on the silicon substrate as the alignment layer. Thereafter, a CF-LCOS microdisplay of VA mode was assembled with a cell gap of 3μm. And a LC mixture, MLC-6608
(ne=1.5578, no=1.4748 and Δε= – 4.2) from Merck, was used for the assembly of the microdisplay. The pretilt angle of the silicon oxide alignment layer on the glass plate was 85º. However, it was very difficult to measure the pretilt angle on the silicon substrate with the color filter array. It was also found that the uniformity of the pretilt angle was poor from the appearance of the microdisplay. It was believed that the silicon oxide layer on top of the color filter array was greatly dispersed and could not maintain uniform pretilt angle. As a result, the VA mode could not be kept up and the microdisplay lost its display function. It was further believed that an improvement of the flatness of the color filter array and increase of the thickness of the silicon oxide layer could improve the stability of the VA mode on the CF-LCOS microdisplays. But it was beyond the scope of this paper. In this paper, emphasis would be placed on the optical modeling and optimization of the CF- LCOS microdisplay of the VA mode.
3. Optical Modeling The optical modeling of the VA mode was more or less the same as that of the TN mode as reported in our previous works . Fig. 1(a) showed the top view of the simulation structure. There were two pixels in the simulation structure and each pixel included three sub-pixels of red, green and blue. The sub-pixels were arranged in delta shape and had a pitch of 10μm by 7.5μm with a pixel gap of 0.5μm. Cross section of the simulation structure was also shown in Fig. 1(b). In this arrangement, the LC cell was driven in frame inversion in which the green sub-pixel was 0V and the red and blue sub-pixels were 4V. The color filter array was 0.75μm thick and the LC cell gap was 3μm in the simulation.
Fig. 1 (a) Top and (b) cross section of the simulation structure. The common voltage on the top electrode was kept at a constant voltage of 5V. As a result, the sub-pixel of 0 and 4V produced a root-mean-squared voltage of 5 and 1V, respectively, across the color filter and LC layers. For a fair comparison with the experimental data, the same LC mixture, MLC-6608 from Merck, was used for the simulation. The simulated director distribution of the VA mode on the CF- LCOS structure was also shown in Fig. 1(b). With the homeotropic alignment, the LC molecules were aligned perpendicular to the surface of the substrate in off-state as shown
ISSN0006-0966X/06/3702-1435-$1.00+.00 © 2006 SID SID 06 DIGEST • 1435
39.2 / B. L. Zhang
by the red and blue sub-pixels in Fig. 1(b). At this state, the LC layer introduced zero birefringence to the incident polarized light, and hence a perfect dark state was resulted through cross polarizers. This good dark state could ensure high contrast of the display. The LC mixtures used in the VA mode had a negative dielectric anisotropy. When an electric field was applied, the LC molecules were lined up and parallel to the surface of the substrate as shown by the green sub-pixel in Fig. 1(b). The simulated spatial optical reflectance of the VA CF-LCOS microdisplay with 88˚ pretilt angle was shown in Fig. 2. In this image, the green sub-pixels were turned. But they were observed with dark disclination lines and divided into four domains with a shape of windmill. The simulated color coordinate of this green image with a LED light source was (0.237, 0.610), which was very good due to very dark red and blue sub-pixels. In comparison, the color coordinates were only (0.247, 0.585) for the MTN mode .
Fig.2 The simulated spatial optical reflectance of the VA CF
LCOS microdisplay. But the brightness of the green image was obviously reduced since the ON region of the bright area did not occupy the whole green sub-pixels. Fig. 3 shows the simulated reflectivity of the color images for both the color MTN and VA CF-LCOS microdisplays. The simulated peak reflectivity of the green image was only 4.7%, which was much smaller than 13% of the MTN mode. The simulated optical reflectance of red and blue images had similar low values. This low optical reflectivity of color images should be improved in order to apply the VA mode to the CF-LCOS microdisplays.
Fig. 3 The simulated reflectivity of the color images for both the
MTN and VA CF-LCOS microdisplays. With an attempt to verify the accuracy of this 3D optical modeling of the VA mode, the simulated spatial optical reflectance was compared with the observed optical reflectance of the CF-LCOS microdisplay sample introduced in Section 2. Fig. 4(a) showed the observed spatial optical reflectance of the VA CF-LCOS microdisplays. It should be noted that the sputtered oxide should produce an 85º pretilt angle on the color filter substrate, but this pretilt angle was difficult to be measured and confirmed. It was
believed that the pretilt angle should be smaller than 85º due to the topography of the color filter array. With the systematic comparisons, we found that the simulation result of 80° pretilt angle, which was shown in Fig. 4(b), coincided with the experimental one very well.
Fig. 4 (a) Observed and (b) simulated spatial optical reflectance of the CF-LCOS microdisplays of VA mode.
4. Optimizations With this 3D optical analysis as a tool, we were able to locate the disclination lines and minimize the color fringing field accordingly. In this section, the color purity and reflectivity of the pixel array were compared with respect to pretilt angle and pixel size. A circularly polarized optical arrangement was proposed to minimize the fringing field of the VA mode.
4.1 Pretilt Angle Pretilt angle is an important parameter to determine the performance of the VA CF-LCOS microdisplays. Contrast ratio, response time, color purity and optical reflectance are all related to the pretilt angle [12-14]. Fig. 5 showed the simulated spatial optical reflectance of the color pixel array with pretilt angle reduced from 90° to 80°. There were four symmetrical LC domains when the pretilt angle was 90°. At this angle, there was no preferable rotational direction for LC molecules when a voltage was applied. As a result, each quadrant has a symmetrical pattern, which was denoted as d1, d2, d3 and d4 as also shown in Fig. 5(a) for easier referring and descriptions later.